More A It includes round, square, octagon, hexagon, and shape wire in coils only for the more commonly used types of stainless steels for general corrosion resistance and high-temperature service. The steel specimens shall undergo the following conditions: 1 annealed as a final heat treatment; 2 cold worked to higher strength; 3 heat treated to an intermediate temper; or 4 heat treated to a hard temper by austenitizing, quenching, and tempering at a relatively low temperature. The materials shall be cold drawn, annealed, and pickled. The steel wires shall conform to the required chemical compositions of carbon, manganese, phosphorus, sulfur, silicon, chromium, nickel, molybdenum, nitrogen, and other elements such as niobium , vanadium, copper, tantalum, titanium and cobalt.
|Published (Last):||2 December 2011|
|PDF File Size:||14.67 Mb|
|ePub File Size:||2.30 Mb|
|Price:||Free* [*Free Regsitration Required]|
A number in parentheses indicates the year of last reapproval. This standard has been approved for use by agencies of the U. Department of Defense. It includes round, square, octagon,hexagon, and shape wire in coils only for the more commonlyused types of stainless steels for general corrosion resistanceand high-temperature service.
The values stated ineach system may not be exact equivalents; therefore, eachsystem shall be used independently of the other. Combiningvalues from the two systems may result in non-conformancewith the standard.
Referenced Documents2. Ordering Information3. Such requirements may include, but are notlimited to, the following End use: machined hydrauliccoupling parts. Material in Condition A may be given a final cold drawing forsize control or finish, or both, slightly raising tensile strength. Current edition approved May 1, Published May Originallyapproved in DOI: S XM 0. S B 0.
S 0. S LC0. S S 0. S Cb 0. S over 0. S A 0. S C 0. AMaximum or range, unless otherwise indicated. Where ellipses appear in this table, there is no requirement and the element need not be analyzed for or reported.
CFor some applications, the substitution of Type L for Type , or Type L for Type , may be undesirable because of design, fabrication, or service requirements. In such cases, the purchaser should so indicate on the order. B cold finished 0. Dia  . A cold finishedannealed95  45  A cold finishedannealed80  35  30 50S A cold finishedannealed  50  40 40S XM A cold finishedannealed  55  35 55S XM A cold finishedannealedB cold finished   5 50S A cold finishedannealedS A cold finishedannealed58  36  20F.
Special bright finishes, lubricant removal, and so forth, forspecial end uses must be negotiated with the producer. Chemical Composition5. Mechanical Requirements6. General Requirements for Delivery7. S A cold finished max  max. AMinimum unless otherwise noted. Where ellipses appear in this table there is no requirement. BYield strength shall be determined by the 0. An alternative method of determining yield strength,based on a total extension under load of 0.
CFor wire products, it is generally necessary to use sub-size test specimens in accordance with Test Methods and Definitions A FElongation requirement for S applies only to diameters greater or equal to 0.
Approved May 1,
Astm A580 Stainless Steel Wire